The influence of substrate temperature on the properties of aluminum-doped zinc oxide thin films deposited by DC magnetron sputtering
- 1k Downloads
Transparent, conducting, aluminum-doped zinc oxide (AZO) thin films were deposited on Corning 1737 glass by a DC magnetron sputter. The structural, electrical, and optical properties of the films, deposited using various substrate temperatures, were investigated. The AZO thin films were fabricated with an AZO ceramic target (Al2O3:2 wt%). The obtained films were polycrystalline with a hexagonal wurtzite structure and preferentially oriented in the (002) crystallographic direction. The lowest resistivity was 6.0 × 10−4Ω cm, with a carrier concentration of 2.7 × 1020 cm−3 and a Hall mobility of 20.4 cm2/Vs. The average transmittance in the visible range was above 90%.
KeywordsSubstrate Temperature Carrier Concentration Hall Mobility Hexagonal Wurtzite Structure Increase Substrate Temperature
Transparent, conductive oxide (TCO) films, primarily indium tin oxide (ITO) films, have been widely applied to the manufacturing of transparent electrodes for flat panel displays, solar cells, organic, light-emitting diodes, integrated optics, piezoelectronic, gas sensor, heat mirror, and surface acoustic wave (SAW) devices due to their high luminous transmittance, good electrical conductivity, good adhesion to substrates, and chemical inertness. However, the high cost of ITO films has motivated efforts to develop alternatives. In particular, aluminum-doped zinc oxide (AZO) thin films, the n-type dopant, have attracted attention as TCO films because of their low resistivity and high transmittance in the visible range. ZnO-based TCOs are relatively inexpensive, and ZnO-based materials also have desirable properties, such as non-toxicity, long-term environmental stability, and excellent infrared ray (IR) shielding .
AZO thin films can be produced by various deposition techniques, including pulsed laser deposition , chemical vapor deposition , sol–gel process , spray pyrolysis , evaporation , and magnetron sputtering . Among the methods, magnetron sputtering has several advantages, such as low processing temperature, good adhesion of films on substrates, very good thickness uniformity, high deposition rates, high density of the films, and the relative ease of scaling to large areas. It is also a simple process, and the process parameters are easy to control.
In this paper, we investigated the influence of substrate temperature on the structural, electrical, and optical properties of AZO thin films, deposited on Corning 1737 glass substrates. AZO thin films were fabricated by DC magnetron sputtering with an AZO ceramic target (Al2O3:2 wt%).
AZO thin films, deposited on Corning glass 1737 (thickness: 0.7 mm) were prepared using a DC magnetron sputtering system. The targets used in this study were sintered stoichiometric ZnO:Al (99.999% purity, 4 mm in diameter, 0.5 mm in thickness). The content of Al2O3 added to the ZnO powder target ranged from 2 wt%. The glass substrates were ultrasonically cleaned in acetone and methanol and rinsed in an ultrasonic bath in deionized water for 10 min, with subsequent drying by nitrogen gas flow before deposition. The sputtering was performed in an Ar atmosphere with a target to substrate distance of 40 mm. An oil diffusion pump with a rotary pump was used to achieve 2.0 × 10−6 mTorr pressure before introducing the Ar gas. The substrate temperature was measured by a thermocouple gauge and a hot cathode gauge. The variation in substrate temperature during the deposition process was maintained within ±5°C. The substrate temperatures used in AZO film deposition ranged from room temperature (R.T.) to 500°C.
The structural, electrical, and optical properties of the AZO thin films were characterized by various techniques. The film thickness was measured, using a surface profiler (Alpha-Step 500, TENCOR, USA) and a field emission scanning electron microscope (FE-SEM, S-4300 Hitachi). A high-resolution X-ray diffractometer (HR-XRD, Bruker D8 DISCOVER, Germany) was used to investigate the crystallinity and crystal orientation of the films. The surface morphology and the surface roughness of the AZO films were examined by atomic force microscopy (AFM, AP0190, Auto-Probe CP Multitask Microscopy). The electrical resistivity, carrier concentration, and Hall mobility were measured at R.T. by the Van der Pauw method. The optical transmittance of the AZO films was measured in the visible range, using an UV–vis NIR spectrophotometer (Japan Shimadzu UV-3101PC). The elemental compositions were investigated by Rutherford back scattering (RBS, NEC 53DH-2) and secondary ion mass spectroscopy (SIMS, PH17200 TOF-SIMS).
3 Results and discussion
3.1 Crystallinity properties
3.2 Electrical properties
3.3 Optical properties
The optical energy gap E g can be obtained from the intercept of (αhυ)2 vs. hυ for direct allowed transition . The optical band gap widths of the AZO films were estimated to be 3.42, 3.44, 3.59, 3.68, 3.62, and 3.60 eV at substrate temperatures of R.T, 100, 200, 300, 400, and 500°C, respectively. The absorption edge of the transmittance shifted to the shorter wavelength (blue-shift) region up to the substrate temperature of 300°C. This result is believed to be due to the Burstein–Moss effect hypothesis. which predicts that the Fermi level inside the conduction band moves upward with increasing donor concentration due to the filling of the conduction band by the increase of electron carriers. It is known that the optical band gap is proportional to the carrier concentration. The optical band gap decreased with increasing substrate temperature above 300°C. These facts correspond with the aforementioned hypothesis.
3.4 Structure and surface morphology
The surface roughness, measured by AFM, of AZO films prepared with different substrate temperatures
Substrate temperature (°C)
The compositions of the AZO thin films, determined using SIMS referenced by RBS, are shown in Fig. 6. The analysis shows that AZO films exhibited a homogenous composition, but the ratio of Zn/O is, in general, greater than 1. This suggests non-stoichiometric structural properties of ZnO . The depth profile of the AZO film resulted in an atomic ratio of Zn/O/Al of 62.27/31.46 /5.93%. The ratio of Al/Zn, by weight, was 1.1%, which is greater than that in the target (2 wt%). This may be due to the sputter yield property of Zn and Al atoms .
AZO films have been deposited by DC magnetron sputtering, with a ZnO target, mixed with 2 wt% Al2O3, on Corning 1737 glass. The objective of this study was to investigate the structural, electrical, and optical properties of thin films, deposited with various substrate temperatures. The obtained films were polycrystalline with a hexagonal wurtzite structure and were preferentially oriented in the (002) crystallographic direction. The lowest resistivity was 6.0 × 10−4Ω cm, with a carrier concentration of 2.7 × 1020 cm−3and a Hall mobility of 20.4 cm2/Vs. The average transmittance in the visible light range was above 90%. In this study, we demonstrated the possibility of producing TCO films based on ZnO with good electrical and optical properties by optimizing the substrate temperature.
This work was supported by Samsung Electronics Co. through the Brain Korea 21 project under the ministry of Education and Human Resources Development.
- 2.J.H. Kim, K-C. Lee, C. Lee, Proc. SPIE Int. Soc. Opt. Eng. 49, 5063 (2003)Google Scholar
- 3.T.M. Barnes, S. Hand, J. Leaf, C.A. Wolden, J. Vac. Sci. Technol. A 22, 2118 (2004)Google Scholar
- 4.M.J. Alam and D.C. Cameron, J. Vac. Sci. Technol. A 19, 1642 (2001)Google Scholar
- 7.B. Huang, S. Wu, J. Li, S. Sun, Z-Q. Tian, Proc. SPIE Int. Soc. Opt. Eng. 152, 5774 (2004)Google Scholar
- 8.C.-H. Park, H.-J. Lee, H.-B. Kim, G.-H. Lee, J. Kor. Inst. Surf. Eng. 38, 188 (2005) Google Scholar
- 13.M. Ohring, Materials Science of Thin Films, 2nd edn. (Academic), p. 176 (2002)Google Scholar